Continuous adsorption of natural organic matters in a column packed with carbon nanotubes
© Naghizadeh et al.; licensee BioMed Central Ltd. 2013
Received: 9 February 2013
Accepted: 16 June 2013
Published: 3 July 2013
In the present study, continuous adsorption experiments were carried out in an adsorption column to survey the efficiency of the carbon nanotubes (CNTs) for removal of natural organic matters (NOMs) from aqueous solution. Parameters such as mass of CNTs, initial NOMs concentration were evaluated and also the breakthrough curves were obtained. Experiments performed with various initial NOMs concentration and various CNTs masses. The breakthrough period was longer at lower initial NOMs concentration. Increase of the initial NOMs concentration, expectedly, resulted in the faster saturation of the CNTs bed. The adsorption capacities for multi wall carbon nanotubes (MWCNT) and single wall carbon nanotubes (SWCNT) in highest initial NOMs concentration were 53.46 and 66.24 mg/g, respectively. The effect of amount of CNTs on breakthrough time and volume of treated water was investigated and resulted that with an increase in the mass of CNTs, breakthrough time occurs very late and the volume of treated water increased. These findings suggested that CNTs present a great potential in removal of NOMs from aqueous solutions.
KeywordsCarbon nanotubes Natural organic matters Adsorption capacity
Natural organic matters (NOMs) is present in all drinking water sources and is a complex mixture of compounds formed from the breakdown of plant and animal material in the environment . NOMs cause problems in the production of drinking water. It has an adverse effect on the aesthetic water quality and may result in biofouling of pipelines with negative hygienic consequence . It has also been demonstrated that the NOM is the basis for the production of the potentially hazardous disinfection by-products (DBPs) . Thus, is has to be removed from drinking water more efficiently.
NOMs can be removed from water by a number of different treatment processes, the most common processes are coagulation and flocculation, ion exchange, nanofiltration, reverse osmosis and adsorption . The major disadvantage of Coagulation and flocculation processes is that NOMs with low molar mass (LMM) and intermediate molar mass (IMM) cannot be removed efficiently when this method is used . On the other hand, slow kinetics is the major restriction in the use of ion exchange process for removal of NOMs. The costs of membrane filtration processes such as nanofiltration and reverse osmosis, however, have been relatively high and its use, therefore, is restricted to special cases .
The discovery of carbon nanotubes (CNTs) by Iijima  added a new member to carbon family. Their novel and unique chemical and physical properties attract many researchers and show a great potential for wide applications such as nanotechnology, electronics, optics, water treatment, and other fields of materials science. The relative large specific surface area (SSA), another important property of CNTs, enables them to become candidate for adsorption of gas , metal ions  and organic compounds .
In the previous study, CNTs have shown exceptional adsorption capability and high adsorption efficiency for various organic contaminants such as dioxin , benzene , 1,2-dichlorobenzene , trihalomethanes  and polycyclic aromatic hydrocarbons (PAHs) .
All these studies mentioned above show that CNTs are promising adsorbents for organic pollutants. The driving forces for interactions between NOMs with activated carbon (AC) and CNTs could be similar since both AC and CNTs are composed of graphene sheets thus similar chemical composition. However, due to distinct arrangement of graphene sheets in AC and CNTs thereby dissimilar surface and structural characteristics, the interaction mechanisms between NOMs and these two types of carbonaceous materials could be different. However, because removal of NOMs by CNTs has rarely been discussed, we carried out this study.
In the present study, multiwall carbon nanotubes (MWCNT) and single wall carbon nanotubes (SWCNTs) were used for NOMs removal. Continuous adsorption experiments were conducted to understand and quantify the effect of influencing parameters such as mass of adsorbent, initial NOMs concentration on breakthrough curve.
CNTs were prepared by Chemical vapor deposition (CVD) method in Research Institute of Petroleum Industry (RIPI), Tehran, Iran. In order to purification and removing the metal nanocatalysts from carbon nanotubes, the final products were dissolving in 37% hydrochloride acid solution for about 16 h at ambient temperature and then washed several times with distilled water until the pH of the solution reached approximately neutral. Treated CNTs were dried in vacuum at 40°C overnight. For eliminate the amorphous carbons, all of the purified CNTs were placed in the furnace at 400°C for 30 min.
A stock solution of 1000 mg/L of NOMs was prepared by dissolving special amounts of humic acid in water. This solution was diluted as required to obtain standard solutions containing 3, 5 and 10 mg/L of NOMs.
First, 500 mL of distilled water was passed through the packed bed to make the packing more compact packing. Stock solutions of NOMs were allowed to flow in down flow mode through the fixed-bed of CNTs controlled by a valve. The parameters varied in the continuous experiments were mass of adsorbent (bed-height), and inlet NOMs concentration. The flow rate was maintained constant using a liquid rotameter (5mL/min). The fixed mass of the adsorbent and the stock solution of initial NOMs concentration were used to maintain the higher accuracy in column experiments. The continuous experiments were carried out at an optimum pH value of 3 obtained by batch experiments.
Where qt is the amount of NOMs adsorbed by CNTs (mg/g), Ac is the area under the breakthrough curve (that was obtained by plotting the adsorbed concentration versus time (t)); Cad is the NOMs adsorbed concentration (mg/L); Q is the flow rate of NOMs solution (mL/min).
Different parameters for the NOMs removal using CNTs in a fixed-bed adsorption column for different operating conditions
Initial NOMs concentration (mg/L)
Break point time parameters
Saturation point time parameters
V bp, mL
t bp, min
q bp, mg/g
V sat, mL
t sat, h
q sat, mg/g
In this study, fixed-bed adsorption studies were used to evaluate the behavior of NOMs removal onto the single and multi wall carbon nanotubes.
Effect of initial noms concentration
According to Figures 1, 2 and 3, as the initial NOMs concentration was increased from 3 to 10 mg/L, the break point time for MWCNT decreased from 900 to 480 min. Also for the SWCNT, as the initial concentration of NOMs was increased from 3 to 10 mg/L, the break point time decreased from 1380 to 720 min. Similar finding have been reported by Gupta and Babu who evaluated the removal of chromium by a fixed bed adsorption column and pointed out that with increasing the initial concentration, the break point time decreased .
The most important criterion in the design of fixed-bed adsorption systems include the estimation of the shape of the breakthrough curve and the appearance of the breakpoint time which determine the operation life span of the bed. Previous study pointed that the breakpoint time is the time of adsorption when the effluent concentration from the column was about 1-5% of the influent concentration .
Regarding to the Table 1 and also according to the total capacity of the CNTs in the column, the total time for adsorption, was found to be decreased from 2460 to 1800 min with an increase in the initial NOMs concentration from 3 to 10 mg/L. Therefore, a change in the initial NOMs concentration has a significant influence on the characteristics of the breakthrough curve. As shown in Table 1 and Figures 1, 2 and 3, with increasing the initial NOMs concentration from 3 to 10 mg/L, the volume of treated water decreased from 4500 to 2400 mL for MWCNT and from 10200 to 3600 for SWCNT.
The increase in the initial NOMs concentration led to reach bed saturation earlier and the break point time was quickly obtained due to the relatively slower transport because of a decrease in diffusion coefficient and the decreased mass transfer coefficient at low NOMs concentration . At higher initial concentration of natural organic matters, adsorption sites quickly saturated and result in decrease in the breakthrough time. It is observed that the adsorbent gets saturated faster at higher concentrations of adsorbate due to the higher rate of adsorbent exhaustion at higher NOMs concentration. On the other hand, for a low initial NOMs concentration, breakthrough occurs very late and the surface of the adsorbents is saturated with NOMs at a relatively longer time. This fact is probably associated with the availability of adsorption sites around or inside the adsorbent particles that are able to capture the NOMs at a lesser retention time. Other studies have also reached to the same results .
As shown in Figures 4 and 5, the longer time needed to reach equilibrium for lower initial NOMs concentration may be explained by the fact that diffusion mechanisms control the adsorption of NOMs onto CNTs. Reid et al. indicated that the mass diffusivity decreases with decreasing concentration under very dilute solution and causes the decrease in diffusion flux of adsorbate onto the surface of the adsorbent . This can be interpreted that if we choose constant mass of adsorbent and constant volume of solution and low concentration of natural organic matters in the solution, therefore, the time needed to adsorbate reached to adsorption sites is higher than when we used high NOMs concentrations.
Effect of carbon nanotubes mass
The amount of CNTs used in the removal of NOMs from aqueous solution is critical for the application of these nonomaterials in NOMs elimination. If the masses of CNTs used in the removal of NOMs are high, then the cost of using CNTs as adsorbent is high and they cannot be used extensively. According to Figure 6 with an increase in the masses of CNTs, the capacities of single and multi wall carbon nanotubes to adsorb NOMs increases which results in a delay to obtain the breakthrough time and also increase in volume of treated water. This may be due to the increase in the adsorbent surface area with increase in the adsorbent amount which provides more binding sites for the adsorption. Other studies have also reached to the same results .
Mechanism of noms adsorption
Different mechanisms may act simultaneously on natural organic chemical and CNT interactions, such as hydrophobic interactions, π-π bonds, electrostatic interactions, and hydrogen bonds. Yang and Xing concluded that the maximum adsorption capacity of a given organic pollutant on CNTs depended on the CNT surface area; surface functional groups on CNTs, the pores in CNT aggregates and surface curvature and defects of CNT monomers . The NOM might provide sterically and electrostatically stable surfaces after adsorption to CNTs. NOMs such as humic acids maybe alter their surface physicochemical properties and enhance their stabilization in water by increasing the steric repulsion and reduce the van der Waals forces between particles.
In this study feasibility of CNTs column adsorption in removal of NOMs was investigated. The parameters such as initial NOMs concentration and CNTs dosage were studied. The results showed that with an increase in the mass of CNTs and initial concentrations of NOMs, the breakthrough time occur very late and the volume of treated water increases. The adsorption capacities of SWCNTs and MWCNTs in removal of NOMs were significant.
The authors greatly acknowledge the Center for Water Quality Research (CWQR), Institute for Environmental Research (IER), Tehran University of Medical Sciences for the support of this research. The authors also gratefully acknowledge Nanotechnology Research Center, Research Institute of Petroleum Industry (RIPI) for the partial support of this work.
- Aiken G, Cotsaris E: Soil and hydrology: their effect on NOM. J Amer Water Works Assoc 1995,87(1):36–37.Google Scholar
- Nordtest: Increase in color and amount of organic matter in surface water, in workshop on changes in quality and quantity of dissolved NOM; causes and cosequenses. Finland: Nordic Council of Ministers; 2003.Google Scholar
- Singer P: Humic substances as precursors for potentially harmful disinfection by-products. Water Sci Technol 1999, 40: 25–30.View ArticleGoogle Scholar
- Crittenden JC, Rhodes TR, Hand DW, Howe KJ, Tchobanoglous G: Water treatment: Principles and design. New York: John Wiley & sons Inc; 2005.Google Scholar
- Matilainen A: Removal of natural organic matter in different stages of drinking water treatment processes. Finland: Tamper university of technology; 2007.Google Scholar
- Liikanen R: Nanofiltration as a refinning phase in surface water treatment, in department of civil and environmental engineering. Helsinki: Helsinki University of technology; 2006.Google Scholar
- Daifullah AAM, Girgis BS, Gad AMH: Study of the factors affecting the removal of humic acid by activated carbon prepared from biomass material. Colloids Surf A 2004, 235: 1–10. 10.1016/j.colsurfa.2003.12.020View ArticleGoogle Scholar
- Han S, Kim S, Lim H, Choi W, Park H, Yoon J, Hyeon T: New nanoporous carbon materials with high adsorption capacity and rapid adsorption kinetics for removing humic acids. Microporous Mesoporous Mater 2003, 58: 131–135. 10.1016/S1387-1811(02)00611-XView ArticleGoogle Scholar
- Lee MC, Snoeyink VL, Crittenden JC: Activated carbon adsorption of humic substances. J Am Water Works Assoc 1981, 73: 440–446.Google Scholar
- Iijima S: Helical microtubules of graphitic carbon. Nature 1991, 354: 56–58. 10.1038/354056a0View ArticleGoogle Scholar
- Cinke M, Li J, Bauschlicher CW, Ricca A, Meyyappan M: CO 2 adsorption in single-walled carbon nanotubes. Chem Phys Lett 2003, 376: 761–766. 10.1016/S0009-2614(03)01124-2View ArticleGoogle Scholar
- Lu C, Chiu H, Liu C: Removal of zinc (II) from aqueous solution by purified carbon nanotubes: kinetics and equilibrium studies. Ind Eng Chem Res 2006, 45: 2850–2855. 10.1021/ie051206hView ArticleGoogle Scholar
- Naghizadeh A, Nasseri S, Nazmara S: Removal of Thrichloroetylene from water by adsorption on to multi wall carbon nanotubes. Iran J Environ Health Sci Eng 2011,8(4):317–324.Google Scholar
- Long RQ, Yang RT: Carbon nanotubes as superior sorbent for dioxin removal. J Am Chem Soc 2001, 123: 2058–2059. 10.1021/ja003830lView ArticleGoogle Scholar
- Tournus F, Charlier JC, Initio A: Study of benzene adsorption on carbon nanotubes. Phys Rev 2005, 165: 421–428. B 71Google Scholar
- Gauden PA, Terzyk AP, Rychlicki G, Kowalczyk P, Lota K, Raymundo-pinero E, Frackowiak E, Beguin F: Thermodynamic properties of benzene adsorbed in activated carbons and multi-walled carbon nanotubes. Phys Lett 2006, 421: 409–414.Google Scholar
- Lu CS, Chung YL, Chang KF: Adsorption of trihalomethanes from water with carbon nanotubes. Water Res 2005, 39: 1183–1189. 10.1016/j.watres.2004.12.033View ArticleGoogle Scholar
- Gotovac S, Honda H, Hattori Y, Takahashi K, Kanoh H, Kaneko K: Effect of nanoscale curvature of single-walled carbon nanotubes on adsorption of polycyclic aromatic hydrocarbons. Nano Lett 2007, 7: 583–587. 10.1021/nl0622597View ArticleGoogle Scholar
- Gupta S, Babu BV: Modeling, simulation, and experimental validation for continuous Cr(VI) removal from aqueous solutions using sawdust as an adsorbent. Bioresour Technol 2009, 100: 5633–5640. 10.1016/j.biortech.2009.06.025View ArticleGoogle Scholar
- American Water Work Association: Standard for Granulated Activated Carbon. Edited by: ANSI/AWWA B604–96. New York: McGraw-Hill Handbooks; 1997.Google Scholar
- Ruthven DM: Principles of Adsorption and Adsorption Processes. Vol. 1. New York: John Wiley & Sons; 1984.Google Scholar
- Goel J, Kadirvelu K, Rajagopal C, Garh VK: Removal of lead (II) by adsorption using treated granular activated carbon: batch and column studies. J Hazard MaterB 2005, 125: 211–220. 10.1016/j.jhazmat.2005.05.032View ArticleGoogle Scholar
- Reid RC, Prausnitz JM, Poling BE: The Properties of Gases & Liquids. Vol. 4. 4th edition. New York: McGraw-Hill; 1988.Google Scholar
- Ren X, Chen C, Nagatsub M, Wang X: Carbon nanotubes as adsorbents in environmental pollution management: A review. Chem Eng J 2011, 170: 395–410. 10.1016/j.cej.2010.08.045View ArticleGoogle Scholar
- Yang K, Xing B: Adsorption of organic compounds by carbon nanomaterials in aqueous phase: Polanyi theory and its application. Chem Rev 2010,110(10):5989–6008. 10.1021/cr100059sView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.